advertisement

International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 08 | Aug 2019 p-ISSN: 2395-0072 www.irjet.net “ANALYSIS OF BEHAVIOUR OF RICE HUSK ASH CEMENT CONCRETE ON ADDITION OF POLYPROPYLENE FIBER” Brijesh Kumar Sahu1, Mr. Bhavesh Kumar Jha2, Mr. Pukhraj Sahu3 M. Tech (Structural Engg.) GEC Jagdalpur Professor, Dept. of Civil Engineering, GEC Jagdalpur, Chhattisgarh, India 3Assistant Professor, Dept. of Civil Engineering, GEC Jagdalpur, Chhattisgarh, India ---------------------------------------------------------------------***---------------------------------------------------------------------2Assistant 1Student, Abstract:- The present day world is witnessing construction in very challenging and difficult circumstances, where a great emphasis is on sustainability. Rice husk ash and polypropylene fiber, by-products of rice mill and textile industry simultaneously, can enhance behaviour of concrete significantly .In this experimental work the objective was to study the effect of rice husk and polypropylene on compressive and split tensile strength of M20 concrete. Rice husk ash and polypropylene have been mixed with concrete in combination in different proportions. Rice husk has been used in 2.5%, 5% &10% by weight of cement. Polypropylene fiber content varies from 0%, 0.25%, 0.5% &0.75% by weight of concrete. We can see the maximum strength value by plotting the test result of cube for compressive strength test and cylinder for split tensile strength test for 7days and 28 days. At 10% rice husk and 0.5% polypropylene 7 days peak compressive strength has been achieved which is 22.6% higher than controlled concrete. At 5% rice husk and 0.5% polypropylene fiber 7 days peak split tensile strength has been achieved which is 53.57% higher than controlled concrete. At 10% rice husk ash and 0.5% polypropylene fiber 28 days peak compressive strength has been achieved which is 54.61% higher than controlled concrete. At 5% rice husk and 0.5% polypropylene fiber 28 days peak split tensile strength has been achieved which is 31.34% higher than controlled concrete. Key Words: Rice Husk Ash, Polypropylene Fiber, Compressive Strength, Split Tensile Strength, ordinary Portland cement (OPC). 1. INTRODUCTION polypropylene fiber has increased tremendously in construction because it behaves like reinforcement. Addition of polypropylene fiber in concrete improves the compressive and tensile strength of concrete. The addition of polypropylene fibers in the concrete significantly affects the compressive strength and split tensile strength of concrete. Addition of polypropylene fiber in concrete increases the compressive strength by 20% to 55% and splitting tensile strength by 30% to 50% respectively. In this study the influence of different amount of rice husk ash and polypropylene fibers content on concrete properties were investigated by measuring compressive strength and splitting tensile strength. 1.1 Objectives The main purpose of this project is to investigate mechanical properties of rice husk ash cement concrete with the addition of polypropylene fiber. Mainly following objectives are considered1. 2. 3. 4. 5. In India, rice milling produces a by product which is also known as husk. Rice husk is a waste material, and has been disposed of by dumping or burning. By using rice husk ash in concrete, we can improve the properties of concrete up to some extent. RHA is found to be good material which fulfils the physical characteristics and chemical composition of mineral admixtures. A small amount of addition of RHA (less than 10 % by weight of cement), is sufficient to improve the durability as well as the strength of concrete. RHA contain high silica content that reduces shrinkage and leads to increases in the strength of concrete 6. To study the properties of fresh and hardened concrete. To study the physical and chemical properties of raw material. To investigate how much percentage of rice husk ash and polypropylene fiber improve mechanical properties of concrete. To study the improvement of split tensile strength of concrete by using rice husk ash and polypropylene fiber. To study the improvement of compressive strength of concrete by using rice husk ash and polypropylene fiber. To study the cost analysis by using RHA and polypropylene fiber. 1.2 Planning For Experiment For this project three types of materials are taken. Mixes are divided into ten batches i.e. (M-1, M-2, M-3, M-4, M-5, M-6, M-7, M-8, M-9 and M-10). Composition of patterns and batches will be same for all work in this project work. Polypropylene fiber are synthetic fiber obtain as a by product from textile industry. Polypropylene fiber is characterized by low specific gravity and low cost. The use of © 2019, IRJET | Impact Factor value: 7.34 | ISO 9001:2008 Certified Journal | Page 388 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 08 | Aug 2019 p-ISSN: 2395-0072 S.N. BATCHES 01. O2. 03. 04. 05. 06. 07. 08. 09. 10. M-1 M-2 M-3 M-4 M-5 M-6 M-7 M-8 M-9 M-10 www.irjet.net DISCRIPTION (CEMENT+RICE RICE HUSK ASH + POLYPROPYLENE FIBER) 100+0+0 97.5+2.5+0.25 97.5+2.5+0.50 97.5+2.5+0.75 95+5+0.25 95+5+0.50 95+5+0.75 90+10+0.25 90+10+0.50 90+10+0.75 Step2. Calculation of target mean strength = 26.6 N/mm² Step3. Calculation or selection of water cement ratio = 0.48 Step4. Calculation of water content = 197.16 litre/m3 Step5. Calculation of cement content = 411kg/m3 Step6. Calculation of mix proportion Mass of coarse aggregate = 1134 kg/m³ Mass of fine aggregate = 670 kg/m³ Step7. Final Mix proportion by weight for trial mix: Water 197 0.48 Cement 411 kg 1 Fine aggregate 670 kg 1.63 Coarse aggregate 1134 kg 2.75 3. TEST ON CONCRETE 3.1 Compressive Strength Test 2. MIX DESIGN The M20 grade concrete generally used for general purpose, For concrete mix design raw material are collected from resources with specified specifications and quality. All the materials are tested as per IS code. In previous time concrete mixed design conforms to IS 456-2000 but in present time with latest provisions concrete mix design calculation has been done as per as per IS 10262-2009. The compressive strength test for concrete specimens has been performed in Compression Testing Machine (CTM) having maximum loading capacity of 2000KN. 30 concrete specimens were tested for 7 days compressive strength and 30 concrete specimens were tested for 28 days compressive strength. Step1. Data required for mix proportioning – S.No. 1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 Characteristic properties Grade of concrete Maximum nominal size of aggregates Grade of cement Specific gravity of fine aggregate Maximum water-cement ratio Workability (for slump test) Grading Zone of fine aggregate Specific gravity of cement Specific gravity of coarse aggregate Aggregate shape Entrapped air Admixture used Maximum temperature of concrete at the time of pouring Minimum cement content Minimum cement content Surface moisture – fine aggregates & coarse aggregates Method of transporting & placing Exposure conditions IS456:2009 Table no 4 © 2019, IRJET | Values M -20 20mm OPC 53 grade 2.65 Fig. 3.1: Compression testing Machine 0.5 100 mm Zone-II 3.15 2.68 Angular 2.00% Nil 27 ± 2°C 3.2 Split Tensile Strength Test The split tensile strength test for concrete specimens has been performed in Split Tensile Testing Machine. 30 concrete specimens were tested for 7 days split tensile strength and 30 concrete specimens were tested for 28 days split tensile strength. 450 kg/m³ 300 kg/m³ Nil Manual Mild Impact Factor value: 7.34 Fig. 3.2: Universal testing Machine | ISO 9001:2008 Certified Journal | Page 389 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 08 | Aug 2019 p-ISSN: 2395-0072 www.irjet.net Sample No % of % of No of cube rice polyp 7 28 husk ropyl days days ash ene test test 1. 0 0 3 3 2. 2.5 0.25 3 3 3. 2.5 0.5 3 3 4. 2.5 0.75 3 3 5. 5 0.25 3 3 6. 5 0.5 3 3 7. 5 0.75 3 3 8. 10 0.25 3 3 9. 10 0.5 3 3 10. 10 0.75 3 3 Sub Total 30 30 Total no of specimen required No of cylinder 7 28 days days test test 3 3 3 3 3 3 3 3 3 3 3 3 3 3 3 3 3 3 3 3 30 30 120 but could reach equal to compressive strength of controlled concrete. 28 days Compressive strength 45 40 Average Compressive Strength (N/mm2) 4. CALCULATION OF NUMBER OF CUBE AND CYLINDER SPECIMEN REQUIRED: 35 30 25 20 0.25% Polypropy lene 15 10 5 0.5% Polypropy lene 0 Percentage of Rice Husk And Polypropylene Fig 5.1.2: 28 Days compressive strength 5. RESULT AND DISSCUSION For 28 days compressive strength the peak strength was obtained as 42.055N/mm2 from concrete containing 10% rice husk ash + 0.5% Polypropylene fiber which was 54.6% higher than compressive strength of controlled concrete (27.2N/mm2). It is also observed that for 0.25% polypropylene fiber + 2.5% rice husk ash compressive strength was significantly higher than controlled concrete. But further increase in rice husk ash percentage compressive strength decreased, but always higher than compressive strength of controlled concrete. For 0.5% polypropylene fiber + 2.5% rice husk ash compressive strength was significantly higher than controlled concrete. But with increase in rice husk ash compressive strength also increased. For 0.75% polypropylene fiber + 2.5% rice husk ash compressive strength was little higher than controlled concrete. But with increase in rice husk ash compressive strength also increased. 5.1 Compressive Strength 7 Days Compressive Strength Average Compressive Strength (N/mm2) 25 20 15 10 5 0 Controlled 2.5% Rice 5% Rice 10% Rice Husk Husk Husk 0.25% Polypropyl ene 0.5% Polypropyl ene 0.75% Polypropyl ene Percentage of Rice Husk And Polypropylene 5.2 Split tensile strength 7 days Split tensile strength For 7 days compressive strength, the peak strength was obtained as 21.37N/mm2 from concrete containing 10% rice husk ash + 0.5% Polypropylene fiber which was 22.6% higher than compressive strength of controlled concrete (17.43N/mm2). It is also observed that for concrete containing 0.25% Propylene fiber + 2.5% rice husk ash, compressive strength was little higher than controlled concrete. But further increase in rice husk ash percentage compressive strength decreased. For 0.5% Polypropylene fiber + 2.5% rice husk ash compressive strength was little higher than controlled concrete. But with increase in rice husk ash, compressive strength also increased. For 0.75% polypropylene fiber + 2.5% rice husk ash compressive strength was lesser than controlled concrete. But with increase in rice husk ash compressive strength also increased © 2019, IRJET | Impact Factor value: 7.34 | 3 Average Compressive Strength (N/mm2) Fig 5.1.1: 7 Days compressive strength 2.5 2 0.25% Polypropy lene 0.5% Polypropy lene 0.75% Polypropy lene 1.5 1 0.5 0 Controlled 2.5% Rice 5% Rice 10% Rice Husk Husk Husk Percentage of Rice Husk And Polypropylene Fig 5.2.1: 7 Days split tensile strength ISO 9001:2008 Certified Journal | Page 390 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 08 | Aug 2019 p-ISSN: 2395-0072 www.irjet.net For 7 days split tensile strength the peak strength was obtained as 2.58N/mm2 from concrete containing 5% rice husk ash + 0.5% Polypropylene fiber which was 53.57% higher than compressive strength of controlled concrete (1.68N/mm2). It is also observed that for 2.5% rice husk ash split tensile strength was lesser than split tensile strength of controlled concrete for every percentage of Polypropylene fiber. For 5% rice husk ash split tensile strength was significantly higher than split tensile strength of controlled concrete for every percentage of Polypropylene fiber. For 10% rice husk ash split tensile strength was lesser than split tensile strength of controlled concrete for all proportions of Polypropylene fiber 28 Days Split tensile strength For 28 days split tensile strength the peak strength was obtained as 3.31N/mm2 from concrete contained 5% rice husk ash + 0.5% Polypropylene fiber which was 31.3% higher than compressive strength of controlled concrete (2.52N/mm2). It is also observed that for 2.5% rice husk ash split tensile strength was lesser than split tensile strength of controlled concrete for every percentage of Polypropylene fiber. For 5% rice husk ash split tensile strength was higher than split tensile strength of controlled concrete for every percentage of Polypropylene fiber. For 10% rice husk ash split tensile strength was significantly lesser than split tensile strength of controlled concrete for every percentage of Polypropylene fiber. Average Compressive Strength (N/mm2) 3.5 ii) iii) iv) v) vi) vii) viii) From above points it is clear that concrete containing 5% rice husk and 0.5% Polypropylene achieves significantly higher characteristic compressive and split tensile strength as compare to controlled concrete with economy. So according to this experimental study the recommended dosage of rice husk and Polypropylene fiber is 5% and 0.5% respectively. REFERENCES 3 1. 2.5 2. 2 0.25% Polypropyl ene 0.5% Polypropyl ene 0.75% Polypropyl ene 1.5 1 0.5 0 3. 4. Controlled 2.5% Rice 5% Rice 10% Rice Husk Husk Husk Fig 5.2.2:of28 Days split strength Percentage Rice Husk Andtensile Polypropylene 5. 6. CONCLUSIONS From all the result and discussions following conclusions can be made:i) Optimum dosage of rice husk can be taken from 5% by weight of cement. Optimum dosage of Polypropylene fiber can be taken from 0.5% by weight of concrete. Maximum increase in compressive strength for 7 and 28 days is 22.6% and 54.61% respectively as compare to control concrete. Maximum increase in split tensile strength for 7 and 28 days is 53.57% and 31.34% respectively as compare to control concrete. For 7 days compressive strength test the concrete containing 0.5% PPF gives greater strength as compare to control concrete for every percentage of RHA. For 28 days compressive strength test the concrete containing 0.25%, 0.5% and 0.75% PPF gives greater strength as compare to control concrete for every percentage of RHA. Cost of per cubic meter concrete containing 5% rice husk + 0.5% polypropylene is Rs2778.44 which is Rs19.1 lesser than cost of per cubic meter controlled concrete. 6. Addition of rice husk and Polypropylene in concrete improves characteristic compressive and split tensile strength. © 2019, IRJET | Impact Factor value: 7.34 | 7. Alsadey Salahaldein (2016) “Effect of Polypropylene Fiber Reinforced on Properties of Concrete” Journal of Advance Research in Civil and Mechanical Engineering. Arivalagan S,(2014) “Earthquake-Resistant Performance of Polypropylene Fiber Reinforced Concrete beams ”, Journal of Engineering and Technology, Vol. 2 (01),pp. 63-67 Aly T Sanjayan G and Collins F,( 2014) “ Effect of Polypropylene Fiber on shrinkage and cracking of concretes”, Journal of materials and structure, Vol. 2 (01) , pp1471-1753 Cengiz, O and Turanil, L (2004). “Comparative evaluation of steel mesh, steel fiber and High performance polypropylene fiber reinforced shotcrete in panel tests”, Cement and Research. Vol.34, Jan .pp 1357-1364. Dave U. V. and Desai Y. M (2007) “ Effect of Polypropylene, Polyester and Glass Fiber on various strength of ordinary and standard concrete”, The First International Conference On Recent Advance in Concrete Technology, Washington D.C.U.S.A. IS: 456-2000, Indian standard, “PLAIN AND REINFORCED CONCRETE CODE OF PRACTICE”, (Fourth Revision). IS: 10262-1982, Indian standard, “RECOMMENDED GUIDELINESS FOR CONCRETE MIX DESIGN”. ISO 9001:2008 Certified Journal | Page 391 8. 9. 10. 11. 12. 13. 14. 15. 16. International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 08 | Aug 2019 p-ISSN: 2395-0072 www.irjet.net IS: 12269-2013, Indian standard, “ORDINARY PORTLAND CEMENT, 53 GRADE-SPECIFICATION” (First Revision). IS: 516-1959, Indian standard, “MEHTOD OF TEST FOR STRENGTH OF CONCRETE” IS: 383-1970, Indian standard, “SPECIFICATION FOR COARSE AND FINE AGGREGATE FROM NATURAL SOURCES FOR CONCRETE” Kishore, R., Bhikshma, V. and Prakash, P.J. (2011) “Study on Strength Characteristics of High Strength Rice Husk Ash Concrete”, Procedia Engineering 14, pp. 266-26 Market study of Polypropylene (3rd edition) Ceresana. Nagrale, S.D., Hazare, H. and Modak, P.R. (2012) “Utilization of Rice Husk Ash”, International Journal of Engineering Research and Applications (IJERA). Vol. 2, Issue 4, pp. 001-005 Shetty, M.S. (2012) Concrete.S. Technology. S. Chand Publication New Delhi. Zhang, M.H., Lastra, R. and Malhotra, V.M. (1996) “Rice Husk Ash Paste and Concrete: Some Aspects of Hydration and the microstructure of the Interfacial Zone between the Aggregate and Paste”, Cement and concrete Research, Vol. 26, No. 6, pp. 963-977. Zhang, M.H., & Malhotra, V. M. (1996) “HighPerformance concrete incorporating Rice Husk Ash as supplementary cementing materials” ACI Materials Journal, 93(6). © 2019, IRJET | Impact Factor value: 7.34 | ISO 9001:2008 Certified Journal | Page 392